27 July 2021 Original Citation:
Electrical control of deep NV centers in diamond by means of sub-superficial graphitic micro-electrodes
(Article begins on next page)
Anyone can freely access the full text of works made available as "Open Access". Works made available under a Creative Commons license can be used according to the terms and conditions of said license. Use of all other works requires consent of the right holder (author or publisher) if not exempted from copyright protection by the applicable law. Availability:
This is the author's manuscript
This full text was downloaded from iris - AperTO: https://iris.unito.it/
iris - AperTO
University of Turin’s Institutional Research Information System and Open Access Institutional Repository from the publishing process - such as editing, corrections, structural formatting, and other quality control mechanisms - may not be reflected in this version of the text. The definitive version of the text was subsequently published in CARBON, 113, 9999,
You may download, copy and otherwise use the AAM for non-commercial purposes provided that your license is limited by the following restrictions:
(1) You may use this AAM for non-commercial purposes only under the terms of the CC-BY-NC-ND license.
(2) The integrity of the work and identification of the author, copyright owner, and publisher must be preserved in any copy.
(3) You must attribute this AAM in the following format: Creative Commons BY-NC-ND license (http://creativecommons.org/licenses/by-nc-nd/4.0/deed.en),
The publisher's version is available at:
When citing, please refer to the published version.
Link to this full text:
Electrical control of deep NV centers in diamond
by means of sub-superficial graphitic micro-electrodes
J. Forneris1,2,3,1, S. Ditalia Tchernij2,1, A. Tengattini2,1,3, E. Enrico4, V. Grilj5, N. Skukan5, G. Amato4, L. Boarino4, M. 5, P. Olivero2,1,3
Istituto Nazionale di Fisica Nucleare (INFN), Sez. Torino, via P. Giuria 1, 10125, Torino, Italy
Physics Department and Inter-departmental Centre - University of Torino; via P. Giuria 1, 10125, Torino, Italy
Consorzio Nazionale Interuniversitario per le Scienze Fisiche della Materia (CNISM), Sez. Torino, Torino, Italy
Istituto Nazionale di Ricerca Metrologica (INRiM); Strada delle Cacce 91, 10135 Torino, Italy
Institute, Bijenicka 54, P.O. Box 180, 10002 Zagreb, Croatia
The control of the charge state of nitrogen-vacancy (NV) centers in diamond is of primary im-portance for the stabilization of their quantum-optical properties, in applications ranging from quan-tum sensing to quanquan-tum computing. In this work buried current-injecting graphitic micro-electrodes were fabricated in bulk diamond by means of a 6 MeV C3+ scanning micro-beam. The electrodes were exploited to control the variation in the relative population of the negative (NV ) and neutral (NV0) charge states of a sub-superficial NV centers ensemble located in the inter-electrode gap re-gions. Photoluminescence spectra exhibited an electrically-induced increase up to 40% in the NV population at the expense of the NV0 charge state, with a linear dependence from the injected cur-rent at applied biases smaller than 200V, and was interpreted as the result of electron trapping at
NV sites. An abrupt current increase at 300V bias resulted in a strong electroluminescence from
the NV0 centers, in addition to two spectrally sharp emission lines at 563.5 nm and 580 nm, not vis-ible under optical excitation and attributed to self-interstitial defects. These results disclose new possibilities in the electrical control of the charge state of NV centers located in the diamond bulk, which are characterized by longer spin coherence times.
The nitrogen-vacancy complex in diamond (NV center) emerged in the last decade as a prominent solid-state quantum system operating at room temperature, and has been exploited for innovative applications in quantum computing and quantum sensing [1-6]. Most of these applications heavily rely on the initialization, manipulation and readout of the spin state of the negatively charged (NV ) state of the defect. However, the NV center is affected by uncontrolled charge state instabilities , thus preventing a coherent spin manipulation of the NV- state before it accidentally converts to the NV0 state .
In recent years, several works addressed the control of the charge state of the NV center by different approaches. The chemical stabilization of NV /NV0 charge state was investigated in shallow centers and nanodiamonds, by means of oxygen [9-11], fluorine  and hydrogen  surface termina-tion. The NV charge state stability has been investigated as a function of laser power and wave-length excitation [7,14,15]. Furthermore, the electrical control was adopted to stabilize the negative charge state of shallow NV centers in a hydrogen-terminated sample [16,17], and to deterministical-ly switch NV centers to the neutral charge state through hole injection in p-i-n devices [18,19]. The charge state control of the NV center by means of electrical pulse sequences is particularly appealing, since it would enable the development of integrated spintronic devices . Despite the recent progresses, the current studies were mainly limited to surface (i.e. <14 nm) defects [16,17] or to the stabilization of the NV0 charge state [18,19], with the exception of the negative charge state
stabilization in p-i-n devices in a sandwich configuration . On the other hand, the possibility of controlling deep NV centers in diamond using flexible electrode geometries would find useful ap-plications in quantum metrology and quantum information processing, since deep sub-superficial NV centers are characterized by significantly longer spin coherence times due to the weaker inter-action with surface defect states .
In this work, the electrical control of the charge state in NV ensembles is investigated in a single-crystal diamond substrate structured with sub-superficial graphitic micro-electrodes fabricated by means of MeV ion beam lithography . The employed fabrication technique allows to define ar-bitrary electrode geometries with micrometric resolution in the diamond bulk (i.e. up to several mi-crometers below the sample surface) by exploiting the radiation-induced graphitization of the mate-rial occurring at the end of the MeV ion penetration range, and has already been successfully adopt-ed to realize different integratadopt-ed devices in diamond, such as bolometers [23,24], particle detectors , cellular biosensors [26,27] and IR emitters . More pertinently to this work, sub-superficial graphitic electrodes were previously employedto stimulate electroluminescence from diamond col-or centers, both in multi-photon  and single-photon  emission regimes. Furthermcol-ore, the exploitation of the ion fabrication technique enabled to investigate the charge state conversion pro-cess by means of non-rectifying ohmic electrodes, thus taking advantage on the related charge in-jection mechanisms.
2.1 Device fabrication
The employed sample was a 3×3×0.3 mm3 single-crystal diamond substrate grown by ElementSix by CVD technique. This optical grade type IIa sample is characterized by nominal concentrations of substitutional nitrogen and boron of <1 ppm and <0.05 ppm, respectively. Two sub-superficial graphitic micro-electrodes were fabricated in the sample bulk by raster-scanning a focused
5 µm 6 MeV C3+ beam along linear paths. The ion fluence ( 4×1016 cm-2) was chosen to
overcome the graphitization threshold  at the end of the ions range, i.e. at a depth of 2.7 µm
below the sample surface, as shown in Figure 1a.
The sample was subsequently annealed at 1000 °C in vacuum for 2 hours to convert the amorphized layer to a graphitic phase. This thermal process was concurrently exploited to induce the formation of a high-density ensemble of NV centers in the gap region comprised between the graphitic chan-nels, due to the aggregation of native nitrogen atoms and the vacancies created by stray ions in the fabrication process. The concentration of induced NV centers in this region can be roughly estimat-ed as follows. A native substitutional nitrogen concentration of 1015 cm-3 was assumed from the manufacturer specification. The density of vacancies induced by the implantation of stray ions in the inter-electrodes gap during the fabrication process is estimated as of 1×1022 cm-3. The V + N
NV conversion efficiency is known to be in the 1-10% range . So, the NV concentration could be estimated in the 10-100 centers µm-3 range. Such values are sufficiently high to prevent the observation of any non-classical feature in the light emission from NV centers, which were in-vestigated as a purely classical ensemble of optically active centers.
Subsequently, the sample underwent a 30 min oxygen plasma treatment (20 sccm O2 flux, 30 W RF power, pressure 2.5×10 2 mbar) with the purpose of removing any residual surface conductivity as-sociated with possible graphitization or contamination occurring during the thermal annealing. In addition, the plasma treatment ensured that the diamond surface was oxygen-terminated, and thus electrically insulating . This feature enabled to investigate unambiguously the electrical conduc-tion features of bulk diamond in the graphitic electrodes gap.
As schematically shown in Figure 1b, 30 keV Ga+ focused ion beam (FIB) milling was performed at the outer endpoints of the micro-channels to expose them to the sample surface. The FIB milling was followed by the deposition of 70 nm thick Ag contacts through a stencil mask, on which elec-trical connections to the external circuit were subsequently wire-bonded. The final device consisted
of two 15 µm wide and 100 µm long graphitic micro-electrodes spaced by a 9 µm gap, as
shown in Figure 1c.
Figure 1: Fabrication of sub-superficial graphitic electrodes in diamond. a) Vacancy-density depth profile
induced by 6 MeV C3+ ions implanted at a fluence of 4×1016 cm-2, as evaluated by SRIM2013.00 Monte Carlo code . The vacancy density exceeds the graphitization threshold in the region highlighted in red, where graphitic electrodes are formed upon thermal annealing. b) Schematic representation of the device: the electrical connections of the graphitic electrodes to the external circuit are fabricated by FIB milling at their outer endpoints, in order to expose them to a subsequent Ag contact deposition and wire-bonding. c) Transmission optical micrograph of the inter-electrode gap region of the fabricated device.
2.2. Electrical and optical characterization
Two-terminal current-voltage (I-V) characteristics were measured with a standard setup (Keitley 6487 picoammeter/voltage source), both in dark conditions and under laser illumination. Increasing voltage steps of 2 V and a constant source time of 300 ms were adopted, both in the acquisition of the I-V curves and of the photoluminescence (PL) spectra from the biased device. The injected
cur-rent was measured during PL acquisitions to monitor the electrical stability of the device. PL meas-urements were performed on the inter-electrode gap region, under different bias conditions. The PL spectra were acquired with a Horiba Jobin Yvon HR800 Raman spectrometer equipped with a 1800 mm-1 diffraction grating ( 0.1 nm spectral resolution). In all the experiments discussed in the
fol-lowing, photoexcitation was provided by a continuous 532 nm laser, with a power of 21.6 mW, as measured on the sample surface. A 20× air objective was employed to define a probed spot region of 3 µm both in diameter and focal depth, i.e. comparable with the penetration range of 6 MeV
C3+ ions in diamond, thus minimizing the effects of possible small stage drifts during the measure-ments at variable bias voltages. To account for slightly non-reproducible focusing conditions, all the reported PL spectra (as well as the combined PL/EL spectra reported in Section 3.3) were normal-ized to the intensity of the first-order Raman peak. Each PL acquisition from the biased device was followed by an acquisition at zero bias voltage, to both verify the absence of residual polarization effects and check the repeatability of the measurements. All measurements were performed in air in a controlled-temperature environment of 20°C.
3. RESULTS AND DISCUSSION
3.1 Electrical characterization
I-V characteristic in dark conditions
The I-V characteristic of the device in dark conditions is reported in Figure 2a (black line). The current measured in these experimental conditions will be referred to as dark current in the fol-lowing. At increasing bias between 0 V and 200 V, a quasi-linear increase of the dark current was observed, indicating an ohmic diamond-graphite interface with a typical resistance value of 700 M [22,35]. The I-V trend exhibited a moderate super-linear current increase at Vbias > 200 V.
with currents larger than 10 µA at 350 V. This behavior was interpreted in terms of Space-Charge-Limited Current (SCLC) caused by the injection of electrons at the ohmic contacts[36,37]. Accord-ingly to this model, the super-linear current increase observed at increasing voltage (i.e. in the 200 300 V range) is associated with the progressive filling of electron traps in the diamond band gap, while the abrupt current increase observed at Vbias > 300 V indicates the complete filling of the
available deep trap states. Such deviation from the ohmic conduction is well described, in the 200-280 V range, by the Mott-Gourney law (to guide the reader s eye, the fitting line is superimposed in blue to the experimental data), describing a quadratic dependence on the applied bias typical of the space-charge-limited current model . Assuming for simplicity a monoenergetical trap distribu-tion in the diamond energy gap, the critical bias Vc = 300 V represents the voltage at which the
elec-tron quasi-Fermi level overcomes the closest deep trap level Et to the conduction band . While
the assumption of an individual type of electron trap in the band gap is rather simplicistic, it is rea-sonable to assume that there is one predominant deep trap level which is responsible for the transi-tion to the high-current-injectransi-tion regime. The positransi-tion of this level in the energy band gap was es-timated according to the SCLC theory , as described below.
Firstly, the following equation expresses the higher threshold value Vc = 300 V:
(1) Vc = q Nt d2 / (2 0 r)
where q is the elementary charge, Nt is the trap density, d = 9 µm is the width of the inter-electrode
gap region, r = 5.5 is the dielectric permittivity of diamond and 0 is the vacuum permittivity. From
Eq. (1), a Nt = (2.2 ± 0.3)×1015 cm-3 value was derived. Considering the 5 µm spot size of the
6 MeV C3+ micro-beam adopted for the device fabrication, the implantation of stray ions with a flu-ence smaller than one order of magnitude in the inter-electrode region is expected . Thus it is reasonable to ascribe the trap density to the residual concentration of ion-induced defects in the ac-tive region of the device after the thermal treatment.
Moreover, the following formula expresses the lower threshold voltage Vtr = 200 V, where a
devia-tion from the linear ohmic conducdevia-tion becomes apparent :
(2) Vtr = 8/9·(q n0 d2)/( 0 r )
where n0 = 8.1×109 cm-3 is the free electron concentration at thermal equilibrium as estimated from
the resistivity (evaluated assuming a 15 µm wide and 3 µm thick active region of the device) of the device at low voltages assuming an electron mobility of µ = 2200 cm2 V1 s1 , and is the ratio between free and trapped electronswhen the electron quasi-Fermi level lies below the trap energy Et . From Eq. (2), a value of = 9.6×10-6,namely the fraction of the total charge density at the
anode which is available for conduction at biases lower than Vtr , was obtained.
Finally, the following formula expresses the value [36,37]:
(3) =Nc/g/Nt·exp(- Et/kT)
where Nc = 1×1020 cm-3 is the effective density of states in the conduction band, g is the degeneracy
of the trap level, Et is the difference between the energy corresponding to the bottom of the
con-duction band and the energy of the trap level, k is the Boltzmann constant and T is the temperature. From Eq. (3), a Et = 0.56 eV was obtained under the assumption of g = 2 (see below) and room
temperature conditions (i.e. neglecting any possible contribution from Joule heating). Indeed, such Et value is in reasonable agreement with the position of the excited state of the NV center, i.e.
0.6 eV from the bottom of the conduction band . On the other hand, also the assumed g = 2 val-ue is compatible with the excited state of the NV center . Thus, we conclude that the electron quasi-Fermi energy at the critical threshold Vc overcomes the excited state of the NV center, so that
all NV centers (and all deeper levels in the band gap) are filled. Consequently, the SCLC model suggests that an almost complete conversion by electron capture from the neutral to the negative charge state of the NV center is achieved at Vbias=Vc (see below for a more detailed discussion).
The I-V trend in high-current-injection regime (i.e., at Vbias > 400 V) is suitably described with a
Poole-Frenkel (PF) model , as demonstrated by the linearization of the asinh(i/V) vs V½ trend (see Figure 2b) deriving from the characteristic PF expression I V sinh(aV1/2/kT) , in good
agreement with previous findings on similar diamond devices . According to this model, the conduction mechanism is dominated by the thermally induced electron emission from traps into the conduction band under the effect of the strong applied electric field . Such exponential depend-ence of the current from the applied bias could hide the quadratic dependdepend-ence of the SCLC conduc-tion mechanism, which is however interpreted as the cause of the abrupt current injecconduc-tion in the ac-tive region of the device. The appearance of a temperature-related current contribution can indeed be regarded as a consequence of the high current density in the small inter-electrode gap. Concur-rently to the transition to this high-current-injection regime, an intense electroluminescence (EL) emission was observed from the inter-electrode gap region. More details on this effect and the above-mentioned interpretation are reported in Section 3.3.
I-V characteristics under laser illumination
I-V curves were also acquired under laser illumination of the inter-electrode gap region of the de-vice (Figure 2, red line) with the same experimental parameters. The current measured in these conditions will be referred to as total current , as it consists of a further contribution ( photocur-rent in the following) arising from photo-generated carriers. A quasi-linear trend in the I-V curve was observed at low bias voltages (<100 V), while a super-linear increase of the total current was apparent at higher voltages. At bias voltages smaller than Vc, the 50% current increase under
Figure 2: a) I-V characteristic in dark conditions (black line) and under laser illumination (red line) of the
inter-electrode gap region. In the inset the data are plotted in linear scale in the 0-200 V range for sake of readability. The blue line, representing the quadratic fit of the dark I-V characteristic in the 200-280V range, evidences that the curve follows the Mott-Gourney law. b) PF electrical conduction in high-current-injection regime. On the basis of the PF formula I V sinh(aV1/2/kT), the data in the 400-450V range are linearized
by suitably re-scaling the quantities reported on the axes.
Moreover, upon laser illumination the transition to a high-current-injection regime was shifted at a higher threshold voltage ( 350 V). This evidence indicates that the optically-induced detrapping of
the carriers represents a competing process with respect to the electron trap filling in the interelec-trode gap, thus supporting the above-mentioned interpretation of the transition between low- and high-current-injection regimes based on the SCLC process.
Figure 3: a) Total current chronogram under variable laser illumination of the inter-electrode gap region, at
an applied bias voltage of 100 V. As schematically shown in the inset, the laser illumination is turned on at time t = 0 s and switched off after 300 s. b) Chronograms of the absolute value of the difference between the measured current and the asymptotic baseline (black lines) in correspondence of the laser turn-on (top) and subsequent switch-off (bottom) together with the corresponding exponential fits (red lines).
The carriers trapping/detrapping mechanisms were further investigated with current measurements under variable laser illumination. As shown in the chronogram reported in Figure 3a, the current in the device biased at 100 V was sampled in concurrence with the turning on and the switching off of the laser illumination, to investigate the related characteristic trapping/detrapping times.
As shown in Figure 3b, both the transitions were characterized by the sum of a fast exponential term and a slower one. In both cases, the former term was associated with a characteristic time smaller than the sampling period (i.e. 300 ms). We ascribed this first component to the trap-ping/detrapping of shallower defects. The slower components of the turn-on and switch-off current transients were characterized by significantly longer decay times, i.e. (65.6 ± 0.4) s and (69.8 ± 0.7) s, respectively. We ascribed this second component to the trapping/detrapping of deep defects in the band gap. These trapping/detrapping effects can be associated with the photo-induced conversion of the charge state of the probed NV centers [14,42], although the possible contribution of other deep levels associated with different defects cannot be ruled out. Temperature-dependent
photocurrent measurements could indeed be useful to further elucidate this issue. It is however worth noting that the measured characteristic PL decay times are significantly shorter than what re-cently reported for trapping/detrapping of the P1 center (i.e. substitutional nitrogen defects) in pho-toconducting diamond , so that at least this possible attribution can be ruled out.
3.2 Charge state conversion
The PL emission from the inter-electrode gap region of the device was measured under different applied bias voltages, with the purpose of assessing the variation of the photophysical properties of the probed NV centers as a function of the injected current between the electrodes. In Figure 4a the PL spectrum from the unbiased device is reported together with PL spectra acquired at increasing bias voltages in the 0 350 V range, i.e. below the transition to the high-current-injection regime (and the concurrent EL emission) is observed. The spectra exhibit the typical PL features of an op-tical grade diamond sample after low-fluence ion irradiation and subsequent annealing, such as the intense first-order Raman peak at 572 nm (corresponding to a 1332 cm-1 Raman shift), and the NV0 and NV zero phonon lines (ZPLs) at 575 nm and 638 nm, respectively, together with their associ-ated phonon sidebands at higher wavelengths . Additionally, the luminescence peak at 740 nm is attributed to residual GR1 centers, i.e. to neutral isolated vacancies . A systematic variation of the relative intensities of the PL features associated with the different NV charge states is clearly visible. For sake of readability, in Figure 4b we report the relative PL spectra acquired from the biased device, i.e. after the subtraction of the reference PL spectrum acquired at zero bias. The most apparent feature of the data displayed in Figure 4b is a substantial decrease in the NV0 emission at increasing bias, concurrently to an increase in the NV emission. It is worth noting that the apparent decrease in the NV ZPL emission is due to the large decrease of the background represented by the NV0 phonon sideband, which results in a lowering of the NV ZPL peak baseline. If the above-mentioned background is subtracted, the intensity of the NV ZPL actually increases with the ap-plied bias, as indicated by the increasing local maximum observed at = 638 nm, and confirmed by
the visible increase in intensity of the NV phonon sideband at higher wavelengths. It is also worth noting that, similarly to the NV0 emission, the GR1 luminescence peak decreases at increasing bias-es, as indicated by the deepening dip at 740 nm.
Figure 4: a) PL spectra acquired from the inter-electrode gap region at increasing applied bias voltages. b)
Relative PL spectra acquired from the biased sample, after subtraction of the reference PL spectrum acquired from the unbiased device.
The quantities A0(i) and A (i) are defined as the values of the integrals of the PL counts calculated
respectively in the 572-580 nm (NV0 ZPL) and 634-642 nm (NV ZPL) spectral intervals. Such values are expressed as functions of the total injected current i and were estimated after the subtrac-tion of their respective baselines. The A0(i) and A (i) values were then normalized to their
respec-tive reference values acquired from the unbiased device, and the resulting A0(i)/A0(0) and
A (i)/A (0) normalized values are reported in Figure 5a as a function of the corresponding injected current. A relative uncertainty of 5% on the ZPL integrals was estimated.
The data reported in Figure 5a exhibit increasing and decreasing linear trends, respectively for the NV (black square dots) and NV0 (red circular dots) normalized ZPL emissions. A quantitative evaluation of the relative concentrations of NV centers in different charge states was performed un-der the assumption that the current-dependent local concentrations of NV0 and NV centers in the
probed region, denoted as n0(i) and n (i), are directly proportional to the correspondent ZPL intensi-ty A0/ (i). Thus it follows that:
(4) n0/ (i) / n0/ (0) = A0/ (i) / A0/ (0)
where the the 0/ subscript refers alternatively to either of the two NV charge states.
Furthermore, we assumed that the probed NV centers only change their charge states between the NV0 and NV ones, i.e. that a possible (and yet to be conclusively demonstrated) population frac-tion of dark NV+ centers remains (if at all present) unchanged under various injection conditions. Such hypothesis is qualitatively supported by the presence of a quasi-isosbestic point in the PL spectra at 655 nm (Figure 4b), at which the emission intensity remains unchanged at increasing
voltages. This observation is in agreement with the lack of conversion from NV0 and NV to an op-tically-inactive NV charge state, whose concentration remains unchanged (if not zero) at all electri-cal biases. Under these assumptions, it follows that the sum of the overall population of NV and NV0 centers (n (i) and n0(i), respectively), is constant for any current flowing in the device:
(5) n (i)+n0(i)=ntot
From the linear fitting in the 0 405 nA range of the n0/ (i)/n0/ (0) vs i data reported in Figure 5a it is possible to express each NV charge state concentration as follows:
(6) n0/-(i) = n0/ (0)·(1+k0/ ·i)
where k0 = ( 0.99 ± 0.03) µA-1 and k = (+1.06 ± 0.06) µA-1 are the respective linear coefficients. From Eqs. (5) and (6) it is possible to obtain, for the unbiased device:
(7) n (0) / n0(0) = | k0 | / k
It follows that n (0) / ntot = (0.52 ± 0.06) and n0(0) / ntot = (0.48 ± 0.06). From these values and the
previously derived linear coefficients it is possible to obtain the relative concentrations of the dif-ferent NV charge states as a function of the injected current (see Figure 5b):
(8) n0(i) / ntot = (0.48 ± 0.06) - (0.48 ± 0.07) · i [µA] n (i) / ntot = (0.52 ± 0.06) + (0.55 ± 0.08) · i [µA]
Figure 5: a) Normalized ZPL intensity from NV (A (i)/A (0), black square dots) and NV0 (A0(i)/A0(0), red
circular dots) centers as a function of the total injected current i. Linear fitting curves of the data in the 0-405 nA range are reported by the continuous lines. b) Variation of n (i)/ntot (black line) and n0(i)/ntot (red
line) as a function of the total injected current i, as resulting from Eq. (8). The dashed lines indicate the un-certainty associated to our estimation, as derived from the fitting procedure.
It is worth noting that a relative concentration of NV centers of n /ntot = (0.74 ± 0.09) is achieved
just below the critical threshold (350 V, 400 nA injected current). Such concentration
corre-sponds to a ~40% increase with respect to the unbiased device. Considering that the steady-state NV relative population n /ntot is always smaller than 0.75 under non-resonant excitation , this
achieved. It is worth remarking that this maximum value is observed in correspondence of the tran-sition to the high-current-injection regime (red curve in Figure 2).
This evidence further supports the interpretation of the charge transport in the device in terms of the SCLC model discussed in Section 3.1. According to this interpretation, the electron trapping occur-ring at the NV centers causes their progressive conversion to the negative charge state; the transi-tion to a high-current-injectransi-tion regime then occurs once all the trap levels are filled. Such interpre-tation is reinforced by the decrease, at increasing voltages, of the GR1 PL emission associated with the neutral vacancy. It is worth noting that such a decrease could be similarly ascribed to the con-version, upon electron trapping, of the vacancy to the negative charge state, which is not optically active under 532 nm laser excitation .
On the other hand, an alternative explanation of the change of the NV charge state based on a varia-tion in the surface electric potential can be ruled out, since a bulk region is probed by means of sub-superficial electrodes. Moreover, it should also be considered that the sample surface was oxidized during the fabrication process to achieve its electrical insulation. While this feature partly contrib-utes to promote the NV negative charge state for the unbiased device [9-11], it however allows to rule out any voltage-dependent chemically-induced shift of the Fermi level occurring below the sur-face of H-terminated diamond [16,17], which is due to electrically-dependent band bending and thus results in the charge state conversion of superficial (i.e. few tens of nm) NV centers. In this way, the electrical control of the NV charge state can be unambiguously attributed to electrical conduction mechanisms occurring exclusively in bulk diamond.
Furthermore, since the injection of a hole current promotes the conversion of the NV centers popu-lation to the neutral charge state , electron trapping/detrapping from/to the conduction band is identified as the predominant process. The occurring of hole trapping/detrapping events cannot be ruled out, but a minority contribution from these processes is expected. This interpretation is based on a unipolar charge transport, and is supported by previous independent experimental results
ob-tained from Ion Beam Induced Charge (IBIC) measurements, where a predominant electron con-tribution to the charge transport properties was observed in the same type of diamond devices . The proposed trapping/detrapping processes associated with electrically-induced NV charge state conversion are: the capture of an electron by an NV0 center resulting in the formation of an NV state  and, conversely, the detrapping of one electron from the NV center to the conduction band, upon either electrical or optical excitation, leading to a switching to the neutral NV0 state [18,38,42]:
(9) a) NV0exc + e NV b) NV exc NV0exc+ e
Consistently with what reported in [14,42], we assume that the electron trapping/detrapping mainly occurs at the excited states (labeled as NV exc and NV0exc in Eq. 9) of the two types of center, due to their closer proximity to the conduction band edge with respect to their respective ground states. In agreement with what discussed in previous works [11,16], the relative increase in the NV concen-tration originates from a shift in the electron quasi-Fermi level, due to the progressive filling of trap states in the band-gap at increasing currents. As highlighted by the electrical characterization dis-cussed in Sect. 3.1, the transition to a high-current regime occurs when the electron quasi-Fermi level reaches the relevant trap state placed at 0.56 eV below the conduction band. Such transition indicates that a complete filling of all the deeper level in the band gap is achieved, including the conversion of the NV centers to the negative charge state by electron capture.
A schematic representation of the concurring electron trapping/detrapping processes responsible for the NV charge state modification in low-current-injection regime is reported in Figure 6. In the fig-ure, the green band represents an excitation energy corresponding to the 532 nm laser from the con-duction band. The electronic transitions of interest are highlighted in green or blue, respectivelt for trapping and detrapping processes.
The diagram represents the energy levels of the ground and excited states of the NV and NV0 cen-ters . In the following, the position of all energy levels is intended as an energy difference from the conduction band. The ground states of the NV and NV0 centers are located at 2.54 eV and 4.3 eV, respectively [16,38]; similarly, the corresponding excited states NV exc and NV0exc lay at 0.6 eV and 2.14 eV . The ground (V0, 2.86 eV) and excited (V0exc, 1.18 eV) states of the GR1 cen-ter, i.e. the neutral single vacancy are also reported . The negatively charged vacancy V (corre-sponding to the ND1 luminescent center) has a ground state placed at 2.6 eV; its excited state V exc (3.15 eV above the ground state) lays within the conduction band .
The following electronic transitions are proposed to play a key role in the charge state modification of the vacancy and of the nitrogen-vacancy center. The conduction of carriers injected at the ohmic diamond/graphite interface occurs mainly within the conduction band. In addition, trap-ping/detrapping phenomena (labeled as 1-4 and 8, 10 in Figure 6) may occur, involving transi-tions to/from the energy levels of the defects from/to the conduction band. The considered detrap-ping/trapping processes can involve shallow traps laying at energy Esh (labeled as 1 and 2 in
Figure 6), the excited state of NV centers labeled as 3 / 4 , as described by Eq. (9), or the
ground state of negative vacancies (labels 10 / 8 , respectively).
The electron detrapping from the NV center results in its conversion to the NV0 state  (labeled as the blue dashed arrows 5 in Figure 6). Conversely, the transition of the NV0 to the negative charge state NV (labeled as the green dashed arrows 6 in Figure 6) is assumed to follow an elec-tron trapping from the conduction band to the available energy level at 0.56 eV, corresponding to the NV exc excited state (transition labeled as 4 in Figure 6).
At increasing electron currents, the progressive filling of the trap states available in the band gap results in an increase in the electron quasi-Fermi level EFn(i) (labeled as the green dashed arrow A
in Figure 6): the NV charge state is then the most favored. Conversely, at decreasing injected cur-rents the electron quasi-Fermi level decreases upon electron detrapping (labeled as the blue dashed arrow B in Figure 6), thus increasing the NV0 population.
Similarly, the decrease in the PL intensity of the GR1 center at increasing currents is interpreted as due to the conversion (labeled as the green dashed line 7 in Figure 6) of the neutral vacancy to the negative charge state. This process, in turn, is a consequence of the non-radiative electron trap-ping from the band gap to the V ground state (green line 8 in Figure 6). The inverse charge state conversion is presented for completeness (dashed blue line 9 in Figure 6) as the result of an elec-tron transition from the V ground state to the conduction band, where its excited state lays (labeled as the blue arrow 10 in Figure 6).
Figure 6: The region highlighted in green indicates the energy levels, which can be optically detrapped upon
532 nm laser excitation (2.33 eV). Schematic representation (in scale) of the electron trapping/detrapping mechanisms occurring in the inter-electrode gap region. Detrapping (labeled as 1 ) and trapping (labeled as 2 ) from/to shallow trap levels at a generic energy Esh contribute to the measured photocurrent (see Figure
neutral charge state (blue dashed line, labeled as 5 ). Conversely, electron trapping at the NVexc level
(green line, labeled as 4 ) causes the conversion of the NV0 center to its negative charge state (green dashed line, labeled as 6 ). Similarly, an electron trapping to (green arrow, label 8 ) or detrapping from (blue ar-row, label 10 ) the ground state of the negative vacancy results respectively in the V0 V (blue dashed line, labeled as 7 ) or V V0 conversion (green dashed line, labeled as 9 ), respectively.
The study of the electrically controlled charge state conversion was limited by the transition to a high-current-injection regime observed at bias voltages higher than 350 V (see Figure 3a). This transition was fully reproducible and stable over multiple excitation cycles. A non-negligible elec-trically induced luminescence was detectable for injected currents larger than 10 µA, i.e. above the transition to the high-current-injection regime, while no EL emission could be detected at lower currents within the experimental sensitivity.
EL was investigated at increasing bias voltages under no laser illumination. An optical micrograph acquired at a bias voltage of 500 V is shown in Figure 7a, exhibiting an intense red emission visi-ble by naked eye in the inter-electrode gap region. EL spectra acquired at 350 V and 500 V bias voltage with the same light collection setup adopted for PL measurements are reported in
Fig-ures 7b and 7c, respectively. The main spectral feature is the emission from the NV0 center, which is clearly characterized by the ZPL at 575 nm and its phonon sidebands at higher wavelengths. The NV emission component is absent from the EL spectrum, consistently with previous reports of the absence of such emission under electrical excitation [19,44]. Moreover, two sharp EL emission lines (not active under optical excitation at 532 nm), are clearly visible at = 563.5 nm and = 580 nm. As shown in Figures 7b and 7c, at increasing injected currents the two above-mentioned EL lines display a similar increase in emission intensity, which is more pronounced with respect to the NV0 emission. Indeed, the NV0 ZPL line is barely distinguishable at 500 V bias (see
= 580 nm lines suggests a possible attribution to the same defect family or to different charge states of the same complex. Although an exhaustive investigation of these previously unreported EL emission lines goes beyond the scope of the present work, they are tentatively attributed to self-interstitial defects, i.e. pairs of nearby self-interstitial atoms along the <100> axis, consistently with what was previously observed in cathodoluminescence and photoluminescence under 488 nm laser excitation, in ion- and electron-irradiated diamonds [44,47].
Figure 7: a) Reflection optical micrograph of the device biased at a voltage of 500 V. The edges of the
(oth-erwise barely visible) graphitic electrodes are highlighted by the white dashed line for sake of clarity. An intense EL emission (circled in red) is clearly visible as the red spot in the inter-electrode gap region. b) EL spectrum acquired from the inter-electrode gap region at a bias voltage of 350 V. c) EL spectrum acquired from the same region at a bias voltage of 500 V.
A quantitative analysis of the EL emission intensity as a function of the injected current was limited by the strong spectral overlap of the NV0 ZPL with the 580 nm emission line. Furthermore, any in-dication on the NV charge state conversion was prevented by the absence of NV emission in EL regime. However, a qualitative analysis of the process was possible by a PL investigation of the de-vice in high-current-injection regime, i.e. at bias voltages higher than 400 V under laser
illumina-tion. In this case, the luminescence spectra acquired in the inter-electrode gap region included both a PL and an EL contribution. The former contribution was associated to the optical excitation of NV0, NV and GR1 centers, while the latter one consisted in the NV0 spectral component and the two afore-mentioned interstitial-related emissions. Figure 8a shows such combined spec-tra acquired at increasing bias voltages (400 V, 450 V and 500 V), while also reporting for compari-son a PL-only emission spectrum acquired from the unbiased device.
At increasing bias voltages, the PL+EL spectra exhibit an increase in the emission intensity over the whole spectral range. The corresponding injected current values can be found in Figure 2a (red curve). Similarly to what reported in Figure 4b, for sake of readability Figure 8b shows the rela-tive" PL+EL spectra obtained after subtraction of the reference spectrum collected from the unbi-ased device.
Firstly, the significant increase in emission intensity from the interstitial-related emission lines at 563.5 nm and 580 nm at increasing bias voltages is clearly visible. On the other hand, as previously mentioned the increase in the NV0 emission is significantly less pronounced with respect to the two afore-mentioned peaks. Nevertheless, a non-negligible increase in the NV0 emission can be appre-ciated by considering the increase in its phonon sidebands. While the overall increase in NV0 emis-sion at increasing injected currents arises in large part from the progressive increase of EL emisemis-sion (see Figures 7b and 7c), it cannot be ruled out that the NV exc NV0exc+ e conversion process is also favored by the underlying electrical conduction mechanism.
On the other hand, the deepening local minimum at = 638 nm indicates that the intensity of the NV emission (and thus the NV centers concentration) decreases at increasing bias voltages in the high-current-injection regime. Remarkably, this trend is opposite to what was observed at bias volt-ages below the critical threshold of 350 V, i.e. a progressive increase in the NV charge state con-centration at increasing voltages (see Figure 4b). It is interesting to notice that such behavior is the same as reported in the study of the charge-state conversion process of NV centers in p-i-n devices
in forward bias . In that case, however, the charge state conversion at biases smaller than the built-in voltage was interpreted in terms of a pure bending of the energy bands.
Finally, it is worth remarking that a significant decrease in the V0 emission is still observed at in-creasing biases, as confirmed by the deepening local minimum observed at = 740 nm. Differently from what observed for the NV emission, this effect is in line with the same trend observed in low current-injection regime (see Figure 4b).
Figure 8: a) PL+EL spectra acquired under laser excitation at increasing bias voltage in the
high-current-injection regime (Vbias = 400-500 V). The PL spectrum acquired from the unbiased device (green line) is also
reported for comparison. b) Corresponding relative luminescence spectra obtained after subtraction of the reference PL spectrum acquired at zero bias.
The observation of EL in a high-current-injection regime dominated by a Poole-Frenkel conduction is somewhat surprising, since the EL emission was previously demonstrated in p-i-n devices to be correlated with electron-hole recombination processes at NV sites, originating from double carriers injection at the electrodes [19,48]. While a hole injection in low-current regime could not be ruled out in first instance, the results discussed in Section 3.2, combined with the previous findings on NV conversion to the neutral charge state upon hole capture , indicate a net contribution to the modification of charge state of the nitrogen-vacancy center which is ascribable to a majority elec-tron current , an interpretation which is fully consistent with previous independent experimental results obtained from Ion Beam Induced Charge (IBIC) measurements in similar devices .
On the other hand, the increasing conversion to the NV0 charge state at increasing bias suggests that the transition to a high-current regime involves the injection of a significantly higher density of holes in the inter-electrodes gap, with respect to the low-current behavior. This interpretation is consistent with previous reports [19,48] on the observation of EL emission in presence of a non-negligible hole component in the high current-injection regime.
Finally, it is worth mentioning that, on the basis of the present results, an interpretation of the ob-tained results in high-current regime exclusively based on a thermally-stimulated trap-ping/detrapping process consistent with the Poole-Frenkel conduction mechanism cannot be ruled out. In this latter interpretation, a high rate detrapping, combined with a high pump electron current can in principle fulfill the same role as the electron-hole injection and recombination in the electri-cal stimulation of the NV0 emission.
4. SUMMARY AND CONCLUSIONS
In this work, we demonstrated that sub-superficial graphitic electrodes can effectively be exploited to control the charge state of nitrogen-vacancy complexes in diamond. The electrical characteriza-tion of the device highlighted an ohmic conduccharacteriza-tion mechanism in the inter-electrodes gap at low voltages; at higher biases (>350 V), a significant current increase was observed and was ascribed, according to the SCLC model, to the filling of traps in the inter-electrodes gap. Such model enabled us to estimate the position of the dominant trap level at 0.56 eV below the conduction band. This value is compatible with the position of the excited state of the negatively-charged NV center. In the low-current-injection regime a linear increase in the NV charge state population at the ex-pense of the neutral charge state NV0 was observed by ensemble PL spectral measurements at in-creasing injected currents. Consistently with the above-mentioned SCLC model, this process was interpreted as the result of trapping of electrons injected in the active region of the device. The elec-trical control of the NV charge state enabled to reach a 75% fraction of negatively charged NV
in the stabilization of the negative charge state at the ensemble level, it cannot be ruled out that such effect is a dynamic result of recurring trapping/detrapping events at individual sites. A clarification on this point will require a thorough investigation at the single-photon emitter level with a confocal setup, involving the fast detection and monitoring of the PL emission of individual NV centers . The high current-injection regime was associated with an intense EL emission. Differently from devices fabricated by He+ ion irradiation , the implantation of C3+ ions prevented the formation of additional color centers related to foreign impurities in the diamond lattice. Interestingly, previ-ously unreported sharp EL emission peaks at 563.5 nm and 580 nm were observed, exhibiting a stronger dependence from the injected current with respect to the NV0 center. These emissions were tentatively attributed to interstitial defects, consistently with previous CL studies [44,47]. Finally, the PL contribution of NV centers in high current-injection regime indicated a decrease in the neg-atively-charged concentration of the NV defect, consistently with an increased hole current injec-tion in the device or, alternatively, with a high-rate thermally-stimulated electron detrapping pro-cess associated with the Poole-Frenkel conduction mechanism.
Apart from shedding light on the fundamental mechanisms underlying charge state modifications of NV centers in diamond, the results reported in this work prospect promising applications in the de-velopment of solid-state devices for quantum technologies applications, where the independent con-trol of individual defects with a large spatial density will be mandatory. These applications will re-quire an improvement in the spatial resolution of the electrodes and a concurrent decrease in the inter-electrode distance. These goals can realistically be achieved by exploiting of already demon-strated advanced ion-beam-lithography techniques basd on implantation masks with sub-micrometric spatial resolution , and should be combined with deterministic implantation and detection techniques [49-51] for the formation of individual defects at pre-selected positions of the device. This would offer the significant advantage of achieving high state conversion efficiency in bulk diamond while significantly reducing the operating voltage and still enabling the spin control of the defects with the utilization of standard surface electrodes. In perspective, these developments
could contribute to stabilize the charge state of deep NV centers preventing an uncontrolled blink-ing. The technique can thus enable the preparation and control of the charge state of deep NV cen-ters (which are known to be characterized by better spin coherence properties with respect to super-ficial defects), thus leading to promising applications in quantum computing and quantum sensing.
This research was supported under the following schemes: project funded by the Italian National Institute of Nuclear Physics (INFN) - CSN5 within the research scheme; Future in Research project (CUP code: D11J11000450001) funded by the Italian Min-istry for Teaching, University and Research (MIUR); - project (CUP code: D15E13000130003) funded by the University of Torino and Compagnia di San Paolo in the
frame-work of the di ricerca di Ateneo scheme; experiment
at the laboratory of INRiM.
 G. J. Milburn, Quantum Measurement and Control of Single spins in diamond, Science 330 (2010) 1188.  D. D. Awschalom, L.C. Bassett, A.S. Dzurak, E.L. Hu, J.R. Petta, Quantum Spintronics: Engineering and Manipulating Atom-Like Spins in Semiconductors, Science 339 (2013)1174.
 H. Bernien, B. Hensen, W. Pfaff, G. Koolstra, M.S. Blok, L. Robledo et al., Heralded entanglement be-tween solid-state qubits separated by three metres, Nature 497 (2013) 86.
 F. Dolde, H. Fedder, M.W. Doherty, T. Nöbauer, F. Rempp, G. Balasubramanian et al., Electric-field sensing using single diamond spins, Nature Physics 7 (2011) 459.
 R.S. Schoenfeld, W. Harneit, Real Time Magnetic Field Sensing and Imaging Using a Single Spin in Diamond, PRL 106, 030802 (2011).
 M. A. Taylor, J. Janousek, V. Daria, J. Knittel, B. Hage, H.-A. Bachor et al., Subdiffraction-Limited Quantum Imaging within a Living Cell, Physical Review X 4, 011017 (2014).
 T. Gaebel, M. Dohman, C. Wittman, I. Popa, F. Jelezko, J. Rabeau et al., Photochromism in single nitro-gen-vacancy defect in diamond, Appl. Phys. B 82, 243 246 (2006).
 M.W. Doherty, N.B. Manson, P. Delaney, F. Jelezko, J. Wrachtrup, L. Hollenberg, The nitrogen-vacancy colour centre in diamond, Physics Reports 528 (2013) 1.
 J. Rondin, G. Dantelle, A. Slablab, F. Grosshans, F. Treussart, P. Bergonzo et al. Surface-induced charge state conversion of nitrogen-vacancy defects in nanodiamonds, Physical Review B 82, 115449 ( 2010).  K.-M. C. Fu, C. Santori, P.E. Barclay, R.G. Beausoleil, Conversion of neutral nitrogen-vacancy centers to negatively charged nitrogen-vacancy centers through selective oxidation, Applied Physics Letters 96 (2010) 121907.
 M.V. Hauf, B. Grotz, B. Naydenov, M. Dankeri, S. Pezzagna, J. Meijer et al., Chemical control of the charge state of nitrogen-vacancy centers in diamond. Physical Review B 83, 081304(R) (2011).
 T.W. Shanley, A.A. Martin, I. Aharonovich, M. Toth, Localized chemical switching of the charge state of nitrogen-vacancy luminescence centers in diamond, Applied Physics Letters 105, 063103 (2014).
 V. Petráková, A. Taylor, I. Kratochvílová, F. Fendrych, J. Vacík, J. et al., Luminescence of Nanodiamond Driven by Atomic Functionalization: Towards Novel Detection Principles, Advanced Func-tional Materials 2012, 22, 812.
 K. Beha, A. Batalov, N.B. Manson, R. Bratschitsch, A. Leitenstorfer, Optimum Photoluminescence Ex-citation and Recharging Cycle of Single Nitrogen-Vacancy Centers in Ultrapure Diamond, Physical Review Letters 109, 097404 (2012).
 Xiang-Dong Chen, C.-L. Zou, F.-W. Sun, G.-C. Guo, Optical manipulation of the charge state of nitro-gen-vacancy center in diamond, Applied Physics Letters 103, 013112 (2013).
 C. Schreyvogel, M. Wolfer, H. Kato, M. Schreck, C.E. Nebel, Tuned NV emission by in plane Al-Schottky junctions on hydrogen terminated diamond, Scientific Reports 4 (2014) 3634.
 B. Grotz, M.V. Hauf, M. Dankerl, B. Naydenov, S. Pezzagna, J. Meijer et al., Charge state manipulation of qubits in diamond, Nature Communications 3 (2012) 729.
 Y. Doi, T. Makino, H. Kato, D. Takeuchi, M. Ogura, H. Okushi et al., Deterministic Electrical Charge-State Initialization of Single Nitrogen-Vacancy Center in Diamond Physical Review X 4, 011057 (2014).  H. Kato, M. Wolfer, C. Schreyvogel, M. Kunzer, W. Müller-Sebert, H. Obloh et al., Tunable light emis-sion from nitrogen-vacancy centers in single crystal diamond PIN diodes, Applied Physics Letters 102, 151101 (2013).
 M. Shimizu, T. Makino, T. Iwasaki, J. Hasegawa, K. Tahara, W. Naruki et al., Charge state modulation of nitrogen vacancy centers in diamond by applying a forward voltage across a p-i-n junction, Diamond & Related Materials 63 (2016) 192.
 T. Staudacher, F. Ziem, L. Häussler, R. Stöhr, S. Steinert, F. Reinhard et al., Enhancing the spin proper-ties of shallow implanted nitrogen vacancy centers in diamond by epitaxial overgrowth, Appl. Phys. Lett. 101 (2012) 212401.
 F. Picollo, D. Gatto Monticone, P. Olivero, B.A. Fairchild, S. Rubanov, S. Prawer et al., Fabrication and electrical characterization of three-dimensional graphitic microchannels in single crystal diamond, New Journal of Physics 14, 053011 (2012).
 A.I. Sharkov, T.I. Galkina, A. Yu Klokov, R.A. Khmelnitskii, V.A. Dravin, A.A. Gippius, High-speed bolometric detector based on a graphitized layer buried into bulk diamond, Vacuum 68 263 (2003).
 T.I. Galkina, A.Y. Klokov, A.I. Sharkov, R.A. Khmelnitskii, A.A. Gippius, V.A. Dravin et al., Bolo-metric Detector Embedded in a Polycrystalline Diamond Grown by Chemical Vapor Deposition, Phys. Solid State 49, 654 (2007).
 J. Forneris, V. Grilj, M. P. Olivero, F. Picollo, N. Skukan et al., Measurement and modelling of anomalous polarity pulses in a multi-electrode diamond detector, EPL 104, 28005 (2013).
 F. Picollo, S. Gosso, E. Vittone, A. Pasquarelli, E. Carbone, P. Olivero et al., A new diamond biosensor with integrated graphitic microchannels for detecting quantal exocytic events from chromaffin cells, Ad-vanced Materials 25, 4696 (2012).
 F. Picollo, A. Battiato, E. Bernardi, L. Boarino, E. Enrico, J. Forneris et al.,Realization of a diamond based high density multi electrode array by means of Deep Ion Beam Lithography, Nuclear Instruments and Methods in Physics Research B 348 (2015) 199.
 S. Prawer, A.D. Devir, L.S. Balfour, R. Kalish, Infrared emission from selected areas in ion-beam-irradiated diamond, Applied Optics 34, 636 (1995).
 J. Forneris, A. Battiato, D. Gatto Monticone, F. Picollo, G. Amato, L. Boarino et al., Electrolumines-cence from a diamond device with ion-beam-micromachined buried graphitic electrodes, Nuclear Instru-ments and Methods in Physics Research B 348 (2015) 187.
 J. Forneris, P. Traina, D. Gatto Monticone, G. Amato, L. Boarino, G. Brida et al., Electrical stimulation of non-classical photon emission from diamond color centers by means of sub-superficial graphitic elec-trodes, Scientific Reports 5 (2015) 15901.
 C. Uzan-Saguy, V. Richter, S. Prawer, Y. Lifshitz, E. Grossman, R. Kalish, Nature of damage in dia-mond implanted at low temperatures, Diadia-mond & Related Materials 4 (1995) 569.
 S. Pezzagna, B. Naydenov, F. Jelezko, J. Wrachtrup, J. Meijer, efficiency of nitrogen-vacancy
centres in New Journal of Physics 12 (2010) 065017].
 S. Szunerits, R. Boukherroub, Different strategies for functionalization of diamond surfaces J Solid State Electrochem (2008) 12: 1205
 J. F. Ziegler, J. P. Biersack, and U. Littmark, The Stopping and Range of Ions in Solids (Pergamon, New York, 2003).
 Y. Chen, M. Hasegawa, H. Okushi, S. Koizumi, H. Yoshida, T. Sakai et al., Electrical properties of graphite/homoepitaxial diamond contact, Diamond Relat. Mater. 11 (2002) 451.
 M.A. Lampert, theory of space-charge-limited currents in an insulator with Phys.
Rev. 103 (1956) 1648.
 F.-C. Chiu, A review on conduction mechanisms in dielectric films, Adv. Mat. Sci. and Engineering (2014) 578168.
 N. Aslam, G. Waldherr, P. Neumann, F. Jelezko, J. Wrachtrup, Photo-induced ionization dynamics of the nitrogen vacancy defect in diamond investigated by single-shot charge state detection, New Journal of Physics 15 (2013) 013064.
 G. Davies, S.C. Lawson, A.T. Collins, A. Mainwood, S.J. Sharp et al., Vacancy-related centers in dia-mond, Phys. Rev. B 46 (1992) 46.
 R. M. Hill, Poole-Frenkel conduction in amorphous solids, Philos. Mag. 23, 59 (1971).
 P.W. May, M.-T. Kuo, M.N.R. Ashfold, Field emission conduction mechanisms in chemical-vapour-deposited diamond and diamond-like carbon films, Diamond & Related Materials 8 (1999) 1490.
 E. Bourgeois, A.Jarmola, P. Siyushev, M. Gulka, J. Hruby, F. Jelezko et al., Photoelectrical detection of electron spin resonance of nitrogen-vacancy centres in diamond, Nature Communications 6 (2015) 8577.  F. J. Heremans, G.D. Fuchs, C.F. Wang, R. Hanson, D.D. Awchalom, Generation and transport of pho-toexcited electrons in single-crystal diamond, Applied Physics Letters 94, 152102 2009 .
 A. M. Zaitsev, Optical properties of Diamond (Springer, New York, 2001).
 P. Olivero, J. Forneris, M. F. Picollo, N. Skukan et al., Focused ion beam fabrica-tion and IBIC characterizafabrica-tion of a diamond detector with buried electrodes, Nucl. Instr. Meth. B 269 (2011) 2340.
 R.S. Sussmann , CVD Diamond for Electronic Devices and Sensors (John Wiley & Sons, 2009).  J. W. Steeds, S.J. Charles, T.J. Davis, A.C. Gilmore, J.M. Hayes, C.D.O. Pickard et al., Creation and mobility of self-interstitials in diamond by use of a transmission electron microscope and their subsequent study by photoluminescence microscopy, Diamond & Related Materials 8 (1999) 94.
 N. Mizuochi, T. Makino, H. Kato, D. Takeuchi, M. Ogura, H. Okushi et al., Electrically driven single-photon source at room temperature in diamond, Nature Photonics 6, (2012) 299.
 J. Riedrich-Möller, S. Pezzagna, J. Meijer, C. Pauly, F. Mücklich, M. Markham et al.,, Nanoimplanta-tion and Purcell enhancement of single nitrogen-vacancy centers in photonic crystal cavities in diamond Applied Physics Letters 106, 221103 (2015).
 D.N. Jamieson, C. Yang, T. Hopf, S.M. Hearne, C.I. Pakes et al., Controlled shallow single-ion im-plantation in silicon using an active substrate for sub- 20 keV ions , Appl. Phys. Lett. 86 (2005) 202101.
 J. B. S. Abraham, B. A. Aguirre, J. L. Pacheco, G. Vizkelethy, E. Bielejec, Fabrication and characteri-zation of a co-planar detector in diamond for low energy single ion implantation , Applied Physics Letters 109, 063502 (2016).